SlideShare verwendet Cookies, um die Funktionalität und Leistungsfähigkeit der Webseite zu verbessern und Ihnen relevante Werbung bereitzustellen. Wenn Sie diese Webseite weiter besuchen, erklären Sie sich mit der Verwendung von Cookies auf dieser Seite einverstanden. Lesen Sie bitte unsere Nutzervereinbarung und die Datenschutzrichtlinie.
SlideShare verwendet Cookies, um die Funktionalität und Leistungsfähigkeit der Webseite zu verbessern und Ihnen relevante Werbung bereitzustellen. Wenn Sie diese Webseite weiter besuchen, erklären Sie sich mit der Verwendung von Cookies auf dieser Seite einverstanden. Lesen Sie bitte unsere unsere Datenschutzrichtlinie und die Nutzervereinbarung.
INTRODUCTIONThe oldest technique for consolidating fibers in a web is mechanicalbonding, which entangles the fibers to give strength to the web.Under mechanical bonding, the two most widely used methods are needle punching and spun lacing (hydroentanglement). Spunlacing uses high-speed jets of water to strike a web so that thefibers knot about one another.The spunlace process can be defined as a nonwovens manufacturingsystem that employs jets of water to entangle fibers and thereby providefabric integrity.Softness, drape, conformability, and relatively high strength are themajor characteristics that make spunlace nonwoven unique amongnonwovens.There are many different specific terms for spunlaced nonwoven likejet entangled, water entangled, and hydroentangled or hydraulicallyneedled but the term, spunlace, is used more popularly in the nonwovenindustry.
Principle This type of bonding employs high speed waterjets to bind the fibers or filaments in a web. Theinteraction of the high energy water jets with thefibers in the web increases the interlacing of thefibers (the interlacement is due to the combinedeffect of the impacting water jets & the waterturbulence created in the web) & produces thedisplacement & the new orientation of parts of thefibers in the web.
Advantages of spunlaceingSpunlaceing technique has some advantages over other techniques, such as: High strength level. High softness, absorbency, permeability(no reinforced points or zones). No use of binders. Ecological harmlessness. High operation speed for web formation & web bonding(500m/min). -Lower production cost. -Higher production output.
MATERIALS USED IN SPUNLACED TECHNOLOGY Most commonly, precursors are mixtures of cellulose and man-made fibers (PET, nylon, acrylics, Kevlar (P84, (imide) etc). In general, cellulosic fibers are preferred for their high strength, pliability, plastic deformation resistance and water insolubility. Cellulosic fibers are hydrophilic, chemically stable and relatively colorless. Another advantage is that cellulose has an inherent bonding ability caused by a high content of hydroxyl groups, which attract water molecules. As the water evaporates from the fabric, the hydroxyl groups on fiber surface link together by hydrogen bonds.
Generally, high micronaire cotton is not recommended for hydro entangled nonwovens because of higher number of neps and small bundles of entangled fibers, resulting in unsightly appearing fabric. In spite of this, fabrics made with lower micronaire fiber show higher strength, probably caused by a higher number of fine fibers and greater surface area.
THE CHOICE OF FIBERS Greige cotton has been used in spun lacing technology. It has been shown that the absorbency rate increases with increasing hydroentangling energy. This is the result of oil and wax removal from the fiber surface. The fiber used in spunlaced nonwoven should have following fiber characteristics: Modulus: Fibers with low bending modulus requires less entangling energy than those with high bending modulus. Fineness: For a given polymer type, larger diameter fibers are more difficult to entangle than smaller diameter fibers because of their greater bending rigidity.
Cross section: For a given polymer type and fiber denier, a triangular shaped fiber will have 1.4 times the bending stiffness of a round fiber. An extremely flat, oval or elliptical shaped fiber could have only 0.1 times the bending stiffness of a round fiber. Length: Shorter fibers are more mobile and produce more entanglement points than longer fibers. Fabric strength, however, is proportional to fiber length; therefore, fiber length must be selected to give the best balance between the number of entanglement points and fabric strength. Crimp: Crimp is required in staple fiber processing systems and contributes to fabric bulk. Too much crimp can result in lower fabric strength and entanglement. Fiber wetability: Hydrophilic fibers entangle more easily than hydrophobic fibers because of the higher drag forces.
Operation Spunlacing is a process of entangling a web of loose fibers on a porous belt or moving perforated or patterned screen to form a sheet structure by subjecting the fibers to multiple rows of fine high-pressure jets of water . Various steps are of importance in the hydroentangling process. The steps characteristic for producing hydroentangled nonwoven fabric include: Precursor web formation Web entanglement Water circulation Web drying
The formed web (usually air-laid or wet-laid, but sometimes spun bond or melt-blown, etc.) is first compacted and prewetted to eliminate air pockets and then water-needled. The water pressure generally increases from the first to the last injectors. Pressures as high as 2200 psi are used to direct the water jets onto the web. It has been argued that 10 rows of injectors (five from each side of the fabric) should achieve complete fabric bonding. Injector hole diameters range from 100-120μm . The holes are arranged in rows with 3-5 mm spacing, one row containing 30-80 holes per 25 mm .
The jets exhaust most of the kinetic energy primarily in rearranging fibers within the web and, secondly, in rebounding against the substrates, dissipating energy to the fibers. A vacuum within the roll removes used water from the product, preventing flooding of the product and reduction in the effectiveness of the jets to move the fibers and cause entanglement. Usually, hydroentanglement is applied on both sides in a step-wise manner. The first entanglement roll acts on the first side a number of times in order to impart to the web the desired amount of bonding and strength. The web then passes over a second entanglement roll in a reverse direction in order to treat and, thereby, consolidate the other side of the fabric. The hydroentangled product is then passed through a dewatering device where excess water is removed and the fabric is dried.
Hydro entanglement carried out at standard conditions ( 1500 psi, web weighing 68 g/m2) requires 800 pounds of water per pound of product. For that reason it is necessary to develop a new filtration system able to effectively supply clean water with this high throughput; otherwise, water jet holes become clogged. This system consists of three stages: Chemical mixing and flocculation, Dissolved air flotation and Sand filtration.
PRECURSOR WEB FORMATION The general properties of web forming from other process are listed as following: Isotropic precursor webs can be produced by air laying system. Carding webs can result in final products, which have higher MD strength than CD strength. Melt blown webs can be produced with good ‘squareness’ of the web. Wet formed webs can especially be produced with good machine direction / cross direction characteristics. The combinations of various types of precursor webs provide numerous options for using in the spunlace process to create various different composites.
WEB SUPPORT SYSTEM (CONVEYOR WIRE) The web support system plays an important part in most nonwoven processes. Especially for the spunlace process, it has a critical role in this process because the pattern of the final fabric is a direct function of the conveyor wire. By special design for the wire, we can have following varied products: Ribbed and terry cloth-like products Aperture products Lace patterns or company logo can be entangled into fabrics Production of composites 3-D fabric formation
THE ENTANGLEMENT UNIT Hydro entanglement is an energy transfer process where the system provides high energy to water jets and then transfers the energy to the precursor. In other words, the energy is delivered to the web by the water needles produced by the injector. Therefore, we can calculate the energy from the combination of the water velocity, and the water flow rate. Flow rate = P½ x D2 x N x 2572 x 10-8 m3/hour/injector/meter Energy = P3/2 x D2 x N x 7 x 10-10 KWH/injector/meter P= water pressure (bar) D=hole diameter (μm ) N= number of holes (per injector per meter) In general, the diameter of water needle ranges from 100 to 170 μm. The highest number of needles is 1666 needles per meter of injector, corresponding to the smaller diameter. The water pressure ranges from 30 bars to 250 bars and it is increased stepwise from injector to injector.
WATER SYSTEM As we know, water is most critical part in spunlace process. Therefore, there are some requirements for the water as follows: Large amount of water- about 606 m3/hr/m/injector for 40 bar and 120 m Nearly neutral pH Low in metallic ions such as Ca No bacteria or other organic materials FILTERATION SYSTEM Due to the large amount of water consumed, the spunlace process requires that it be recycled. Therefore, a high quality filtration system is necessary for the spunlace process. Some of special filters are listed as following: Bag filter Cartridge filter Sand filter
WEB DRYING When the fabric leaves the entanglement zone the web, it is completely saturated with water. There are a few steps to remove water from the fabric. The include: Vacuum dewatering system Drying system
PROPERTIES OF SPUNLACED FABRICS Spunlaced fabrics show high drape, softness and comfortable handle( because more fiber entanglement leads to increased strength without an increase in shear modulus. Shear modulus remains low and is virtually independent of the degree of entanglement . The softness of the fabric is explained by the fact that the entangled structures are more compressible than bonded ones, as well as having mobility and partial alignment of fibers in the thickness direction. Good dimensional stability, which is also accountable for drape, softness, and good strength/weight properties of the fabric, pilling and abrasion behavior. The strength of hydroentangled fabrics is lower than that of woven and higher than that of knitted fabrics, whereas the wash durability is considerably lower than that of woven or knitted fabrics.
APPLICATIONS Spunlace fabrics can be further finished, usually dyed and/or printed, treated with binders to allow for wash durability, or fire retardants can be applied to resist burning. The fabric can be treated by antimicrobial agents to enhance resistance against microorganisms. Surgical packs and gowns. Protective clothing as chemical barriers to wipes. Towels and Sponges for industrial, Medical, Food service and consumer applications. The main reason for wide use of these fabrics in medical applications is based on relatively high absorption abilities. Another important criterion is absence of a binder in the fabric allowing sterilization of the fabric at high temperatures. Bacteria-proof Cloth. Cleaning Cloth .
Wet tissues Make up cottonBacteria proof cloth Cleaning cloth Magic Towel
APPLICATIONS Magic Towel. It has no formaldehyde and gluey substances. Thats good for your health and convenience. Easy to carry out for picnic, travel, and even as promotion gifts. One can print their LOGO on the tag for advertisement. Wet Tissue Processed by the advanced high-pressure-water method. The nonwoven spunlace has no Formaldehyde. No glue-like substance, tender the soft skin. For the refreshing experience, it is comfortable for body and parents like it. The wet tissue is used for make-up, make-up removal, and other facial applications. In fact, it is convenient all the day.
Make -up Cotton Hi-Tech Nonwoven Spunlace which has no any chemical substance, but does have a soft touch and is tender to baby skin. Saving the lotion and make-up cream. Best absorption, No fluffed cotton. Best use for make up, wiping lips-sticker, fingernail polish, glasses, leather, jewels, and so on.
Reference….1. Suzuki, M.: New Nonwoven and its Technical Features, INDEX 84 Congress, Session 2 Component and Process developments, Geneva, 19842. A Paper published on “Spunbonding and Spunlacing Two leading technologies coming together”3. By Alfred Watzl; Vice President; Fleissner GmbH & Co4. SPUNLACE (HYDROENTANGLEMENT) Updated: April, 2004 - M. G. Kamath, Atul Dahiya, Raghavendra R. Hegd (Hsu-Yeh Huang & Xiao Gao)5. Hand book of nonwovens6. http://www.jacob-holm.com/technology.html7. http://www.cotteninc.com